Disclosure to Promote the Right To Information Whereas the Parliament of India has set out to provide a practical regime of right to information for citizens to secure access to information under the control of public authorities, in order to promote transparency and accountability in the working of every public authority, and whereas the attached publication of the Bureau of Indian Standards is of particular interest to the public, particularly disadvantaged communities and those engaged in the pursuit of education and knowledge, the attached public safety standard is made available to promote the timely dissemination of this information in an accurate manner to the public. “जान1 का अ+धकार, जी1 का अ+धकार”
“प0रा1 को छोड न' 5 तरफ”
“The Right to Information, The Right to Live”
“Step Out From the Old to the New”
Mazdoor Kisan Shakti Sangathan
IS 4031-1 (1996): Methods of physical tests for hydraulic cement, Part 1: Determination of fineness by dry sieving [CED 2: Cement and Concrete]
“!ान $ एक न' भारत का +नम-ण” Satyanarayan Gangaram Pitroda
“Invent a New India Using Knowledge”
“!ान एक ऐसा खजाना > जो कभी च0राया नहB जा सकता ह” है” ह Bhartṛhari—Nītiśatakam
“Knowledge is such a treasure which cannot be stolen”
IS4031(Part1):1996 ( Reaffirmed 2005 )
Indian Standard METHOD OF PHYSICAL TESTS FOR HYDRAULIC CEMENT PART 1 DETERMINATION OF FINENESS BY DRY SIEVING
BUREAU OF INDIAN STANDARDS MANAKBHAVAN, 9 BAHADUR SHAH ZAFAR MARG NEW DELHI 110002 Price Group 2
Cement and Concrete Sectional Committee, CED 2
FOREWORD This Indian Standard (Second Revision) was adopted by the Bureau of Indian Standards, after the draft finalized by Cement and Concrete Sectional Committee had been approved by Civil Engineering Division Council. Standard methods of testing cement are essential adjunct to the cement specifications. This standard in different parts lays down the procedure for the tests to evaluate physical properties of different types. of hydraulic cements. The procedure for conducting chemical tests of hydraulic cement is covered in IS 4032 : 1985 ‘Methods of chemical analysis of hydraulic cement ( first revision )‘. Originally all the tests to evaluate the physical properties of hydraulic cement were covered in one standard but for facilitating the use of this standard and future revisions, the revised standard was brought out in different parts, each part covering different tests. This part covers determination of fineness of cement by dry sieving. The second revision of this standard has been prepared with a view to align this test method with European S!andard EN 196 (Part 6) Method of testing cements: Determination of fineness. The composition of the Committee responsible for the formulation of this standard is given at Annex A. For the purpose of deciding whether a particular requirement of this standard is complied, the final value, observed or calculated, expressing the result of a test or analysis, shall be rounded off in accordance with IS 2 : 1960 ‘Rules for rounding off numerical values ( revised )‘. The number of significant places retained in the rounded off value should be the same as that of the specified value in this standard.
IS 4031 (Part 1) : 1996
Indian Standard METHOD OF PHYSICAL TESTS F<OR HYDRAULIC CEMENT PART 1 DETERMINATION OF FINENESS BY DRY SIEVING ( 1
Second Revision )
cylindrical frame of 150 mm to 200 mm nominal diameter and 40 mm to 100 mm depth, fitted with 90 pm mesh sieve cloth of woven stainless steel, or other abrasion-resisting and non-corrodible metal wire.
1.1 This standard (Part 1) covers the procedure for determining the fineness of cement by dry sieving as represented by the mass of residue left on a standard 90 w IS Sieve.
The sieve cloth shall comply with the requirements of IS 460 ( Part 1) : 1985 and IS 460 ( Part 3 ) : 1985 and shall be free of visible irregularities in mesh size when inspected optically by the methods of IS 460 ( Part 3 ) : 1985. A tray fitting beneath the sieve frame and a lid fitting above it shall be provided to avoid loss of material during sieving.
2 REFERENCES 2.1 The following Indian Standards are necessary adjuncts to this standard: IS No.
460 ( Part 1 ) : 1985
for test sieves:
Capable of weighing up to 10 g to the nearest 10 mg.
Wire cloth test sieves (third revision)
( Part 3 ) : 1985
Methods of examination of apertures of test sieves (third
A nylone or pure bristle brush, preferably with 25 to 40 mm bristle, for cleaning the sieve.
3535 : 1986
Methods of sampling hydraulic cements (f?rst revision)
5165 : 1969
Interchangeable conical ground - glass joints
4.3 Material for Checking the Sieve A Standard reference material of known sieve residue shall be used for checking the sieve. The material shall be stored in sealed, airtight containers to avoid changes in its characteristics due to absorption or deposition from the atmosphere. The containers shall be marked with the sieve residue of the reference material.
3.1 The samples of the cement shall be taken according to the requirements of IS 3535:1986 (see 2.1) and the relevant standard specification for the type of cement being tested. The representative sample of the cement selected as above shall be thoroughly mixed before testing.
4.4 Procedure 4.4.1 Determination
Agitate the sample of cement to be tested by shaking for 2 min in a stoppered jar to disperse agglomerates. Wait 2 min. Stir the resulting powder gently using a clean dry rod in order to distribute the fines throughout the cement.
4 SIEVING METHOD 4.1 Principle The fineness of cement is measured by sieving it on standard sieve. The proportion of cement of which the grain sizes are larger than the specified mesh size is thus determined.
Fit the tray under the sieve, weigh approximately 10 g of cement to the nearest 0.01 g and place it on the sieve, being careful to avoid loss. Disperse any agglomerates. Fit the lid over the sieve. Agitate the sieve by swirling, planetary and linear movement until no more fine material passes through it. Remove and weigh the residue. Express its mass as a percentage, R,, of the quantity first placed in the sieve to the nearest 0.1 percent. Gently brush all the fine material off the base of the sieve into the tray.
A reference sample having a known proportion of material coarser than the specified mesh size is used for checking the specified sieve. 4.2 Apparatus 4.2.1 Test Sieve It comprises a
of the Cement Residue
Repeat the whole procedure using a fresh 10 g sample
IS 4031 (Part 1) : 1996
repeat determination of residue to yield two values p, and P, expressed to the nearest 0.1 percent.
to obtain 5. Then calculate the residue of the cement R as the mean of R, and R, as a percentage, expressed to the nearest 0.1 percent.
The two values of P, and P, for a satisfactory sieve should differ by not more than 0.3 percent. Their mean P characterizes the state of the sieve.
When the results differ by more than 1 percent absolute, carry out a third sieving and calculate the mean of the three values.
Given the known residue on the 90 m mesh of the reference material, R, calculate R/P as the sieve factor, F, expressed to the nearest 0.0 1. The residue, R, determined as in 4.4.1 shall be corrected by multiplying by F, which may have a value of 1.00 + 0.20
The sieving process is carried out manually by a skilled and experienced operator. NOTE - Alternatively a sieving machine may be used provided that it can be shown to give the same results as the manual operation.
Check the sieve after every 100 sievings. 4.4.2 Checking
NOTE - Any other checking procedure, such as the optical methods described in IS 460 ( Part 3 ) : 1985 may be used. All sieves will wear slowly and consequently their sieve factor, F, will slowly change.
Agitate the sample of cemem LObe tested by shaking for 2 min in a stoppered jar to disperse agglomerates. Wait 2 min. Stir the resulting powder gently using a clean dry rod in order to distribute the fines throughout the cement.
eport the value of R, to the nearest 0. Ipercent, as
Fit the tray under the sieve. Weigh approximately 10 g of the reference material to the nearest 0.01 g and place it in the sieve, being careful to avoid loss. Carry out the sieving procedure as in 4.4.1 including the
t e residue on the 90 pm sieve for the cement tested. % The standard deviation of the repeatability is about 0.2 percent and of the reproducibility is about 0.3 percent.
ANNEX A ( Foreword ) COMMITTEE
Cement and Concrete Sectional Committee, CED 2 Represenfing
In personal capacity ( University of Roorkee# Roorkee
247 667 )
Members SHRI H. BHATTACHARYA SHRI G. R. BHARTIKAR DR A. K. CHAITERJEE SHRI S. H. SUBRAMANIAN ( Alternaie ) CHIEF ENGINEER(DESIGN ) SUPERI~JTENDMG ENGINEER,( S&S ) ( Alternate ) CHIEFENGINEER,NAVAGAM DALU( SUPER~NTENDMG ENGINEER,QCC (Alternate ) CHIEFENGINEER, RESEARCH-CUM-DIRECTOR RESEARCHOFFICER, CONCRETETECHNOLOGY ( Alternate ) DIRECTOR JOINTDIRECTOR( AItemate ) DIRECTOR(CMDD) ( N&W ) DEPUTYDIRECTOR( CMDD ) ( NW&S ) ( Alternate ) SHRI K. H. GANGWAL SHRI V. P~ABHI ( Alternate ) SHRI V. K. GHANEKAR
Orissa Cement Limited, New Delhi B.G. Shirke & Co, Pune The Associated Cement Companies Ltd, Bombay Central Public Works Department, Sardar Sarovar Narmada Nigam Irrigation and Power
New Delhi Ltd, Gandhinagar
Research Institute, Amritsar
A.P. Engineering Research
Central Water Commission,
Hyderabad Industries Ltd, Hyderabad Structural Engineering
Research Centre (CSIR), Ghaziabad ( Continued on page 3 )
IS 4031 (Part 1) : 1996 ( Continued from
2 ) Repnzsenting
SHRI R. TAMILAKARAN ( Alternate SHRI
S. K. GUHA THAKURTA SHR~ S. P. SANKARANARAYANAN ( Alternate )
SHRIN. S. BHAL DR IRSHADMASOOD(
& Co Ltd, Bombay
( CSIR ), Roorkee
of India, New Delhi
Research, Designs Lucknow
Indian Hume Pipes Co Ltd, Bombay National
Test House, Calcutta
Larsen and Toubro Limited, Structural
( CSIR ), Madras
Ltd, New Delhi
Ministry of Transport, Department of Surface Transport New Delhi Central Board of Irrigation and Power, New Delhi
SHRI S. K. NATHANI, SO I DR A. S. GOEL, EE (Alternate
SHRIy. R. PHULL
( CSIR ), New Delhi
ShRl Y.R. PHULL SHRIA.K. SHARMA( Alternate ) DR C. RAJKUMAR DR S. C. AHLWALIA ( Alternate ) SHRIG. hMDAS SHRIR. C. &ARM
JOINT,,DIRECTORSTANDARDS( B&S )( CB-II ) ( Alternate ) SHRI N. G. JOSHI SHRI P. D. KELKAR ( Alternate ) SHR, D. K. KANUNGO SHRI B. R. MEENA ( Alternate ) SHRI P. KRISHNAMURTHY SHRI S. CHAKRAVARTHY ( Alternate ) DR A. G. MADHAVARAO SHRI K. MANI (Alternate ) SHRI G. K. MAJIJMDAR SHRI J. SARIJP( Alternate ) SHRIPUFULLA KUMAR SHRI P. P NAIR ( Alternate ) MEMBER SECRETARY
SHRIS. S. SEEHRA(
DR IRSHAD MASOOD SHRIN. C. J~JN(Alternate) JOINTDrsscro~ STANDARDS ( B&S )( CB-I )
DIRECTOR ( CIVIL ) (
The India Cements
Indian Roads Congress, National
for Cement and
SHRIS. A. REDDI REPRESENTATIVE
Gammon India Ltd, Bombay Builderâ€™s Association of India, Bombay Geological Survey of India, Calcutta
SHRI J. S. SANGANEW SHRIL. N. AGARWAL(
SHRIS. B. SURl
Soil and Materials,
SHRI N. CHANDRASEKARAN( Alternate ) SUPERINTENDING ENGINEER ( DESIGN) EXECUTIVEENGINEER (S. M. R. DMSION )
Public Works Department,
of Tamil Nadu,
(Alternate) SHRIA. K. CHADHA
SHRI J. R. SIL (Alternate ) DR H. C. VISVESVARAYA SHRI D. C. CHATURVEDI ( Alternate ) SHRIVINODKUMAR Director ( Civ Engg )
Prefab Ltd, New Delhi
The Institution Director
( India ), Calcutta
BIS ( Ex-officio Member )
MemberSecretary SHRLJ.K. PRASAD
( Continued on page 4 ) 3
IS 4031 (Part 1) : 1996 ( Continued from page 3 )
Composition of Cement, Pozzolana and Cement Additives Subcommittee, CED 2 : 1 Representing
Convener DR H. C. VISVESVARAYA
( University ofRoorkee, Roorkee 247 667 )
Members SHRI. B. R. MEENA SHFL B. K. &NDAL ( AJtemate ) SHRI N. G. BASAK SHIU T. MADNESHEAR (Alternate ) SHRI SOMN~H BANERIEE CHIEF ENGINEER( RESEARCH-CUM-DIRECTOR) RESEARCHOFFICER (CONCRETETECHNOLOGY)
Test House, Calcutta
Cement Manufacturerâ€™s Association,Bombay Irrigation Department,Government of Punjab
(Alternate) DIRECTOR SHRI J. K. PANEL( Alternate ) DIRECTOR RESEARCHOFFICER ( Alternate ) DIRECTOR(CLMDD II) ,DEPUT~ DIRECTOR( CLMDD II ) ( Alternate ) SHRI R. K. G.XITANI DR R. K. &ID ( AJtemate ) DR A. K. CH~UTERJEE SHRI C. H. PAGE ( AJtemate ) DEPUTYDIRECTOR( B&F ) ASSISTANTDESIGN ENGINEER( Alternate ) SHR~V K. MEHTA SHRI U. B. DANGI ( Alternate ) SHRI G. K. MAJUMDAR DR IRSHAD MASSED SHRI S. K. GARG ( Alternate ) SHRI R. KUNJITHAP~~ EXEC~I-I~E ENGINEER SHRI K. NARANAPPA SHR~ D. P. KEWALRAGMANI(Alternate ) DR S. C. AHLUWALIA SHRI K. H. BABU ( AJtemate ) SHRI M. K. MUKHERJEE SHRI N. K. S~HA ( AJtemate ) SHRI J .D. DESAI SHIU B. K. JAG( AJtemate ) SHRI y. R. PHULL SHRI S. S. SEEHRA( Alternate ) DR K. C. NARANG SHRIC. S. SHARMA(Alternate ) SHlu PuRAM MAL SHRI K. M. NAMB~AR( AJtemate ) SHRI S. A. REDDI PROJECT DIRECTOR SHRI M. P. SINGH SUPERRJTENDMG ENGINEER( D ) SENIORDEPIJIY CHIEF ENGINEER( GENERAL ) (Alternate ) SHRl S. B. SURI SHRI N. CHANDRASEKARAN ( AJtemate ) SHRI L. SWA~XIP SHRI H. BHATTACHARYE ( Alternate ) SHRI D. P. CHAKRAWAKtl SHRI RAJAN C. M~~~HAw( AJtemate )
Central Water Commission, Shree Digvijay The Associated Research,
Cement Co Ltd, Bombay Cement Company
Ltd, Bombay Organization,
Co Ltd, Bombay
Hospital Services Consultancy Corporation (India) Ltd, New Delhi Central Building Research Institute (CSIR), Roorkee Vishnu Cement Ltd, Hyderabad Central Warehousing Corporation, New Delhi Central Electricity Authority, New Delhi National
Council for Cement and Building
Road Wing, Department
Gujarat Ambuja Cement, Ahmedabad Central
Road Research Institute, New Delhi
Dalmia Cement (Bharat) Ltd, New Delhi Engineer-in-Chiefs
Branch, Army Headquarters, New Delhi
Gammon India Ltd, Bombay Cement Corporation of India Ltd, New Delhi Federation of Mini Cement Plants, New Delhi Public Works Department, Government of Tamil Nadu
Central Soil L Materials Research Station, New Delhi Orissa Cement Ltd. New Delhi Bhilai Steel Plant. Bhilai
Bureau of Indian Standards BIS is a statutory institution established under the Bureau oflndian StandardsAct. 1986to promote harmonious development of the activities of standardization, marking and quality certification of goods and attending to connected matters in the country. Copyright BIS has the copyright of all its publications. No part of these publications may be reproduced in any form without the prior permission in writing of BIS. This does not preclude the free use, in the course of implementing the standard, of necessary details, such as symbols and sizes, type or grade designations. Enquiries relating to copyright be addressed to the Director (Publications), BIS. Review of Indian Standards Amendmehts are issued to standards as the need arises on the basis of comments. Standards are also reviewed periodically; a standard along with amendments is reaffirmed when such review indicates that no changes are needed; if the review indicates that changes are needed, it is taken up for revision. Users of Indian Standards should ascertain that they are in possession of the latest amendments or edition. This Indian Standard has been developed from Dot No. CED 2 ( 5168 ).
Amendments Issued Since Publication Amend No.
Date of Issue
Headquarters : Manak Bhavan, 9 Bahadur Shah Zafar Marg, New Delhi 110002 Telephones : 323 01 31,323 94 02, 323 83 75
Telegrams: Manaksanstha ( Common to all offices ) Telephone
Regional Offices: Central : Manak Bhavan, 9 Bahadur Shah Zafar Marg NEW DELHI 110002 Eastern : l/14 C. I. T. Scheme VII M, V. I. P. Road, Maniktola CALCUTTA 700054 Northern : SC0 335-336, Sector 34-A, CHANDIGARH 160022 Southern : C. I. T. Campus, IV Cross Road, MADRAS 600113 Western : Manakalaya, E9 MIDC, Marol, Andheri (East) MUMBAI 400093
32376 17 323 3841 3378499,3378561 337 86 26,337 86 62 60 38 43 I 60 20 25 235 02 16,235 04 42 235 15 19,235 23 15 8329295,8327858 1 8327891,8327892
BHUBANESHWAR. BHOPAL. Branches : AHMADABAD. BANGALORE. HYDERABAD. GHAZIABAD. GUWAHATI. COIMBATORE. FARIDABAD. PATNA. THIRUVANANTHAPURAM. JAIPUR. KANPUR. LUCKNOW. i Pnnted at New India Printing Press,